Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.6, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications12Preparation and Characterization of Poly (2-hydroxyethylmethacrylate) (PHEMA) Nanoparticles with Possible Applications inControlled Drug DeliveryHuda Khan, A.K.Bajpai and R.N.ShuklaSamrat Ashok Technological Institute, Vidisha (M.P)Ziahudakhan.firstname.lastname@example.orgAbstractThe present work describes preparation, structural and morphological characterization of PHEMA nanoparticles. It isfound that the nanoparticles are having size up to 100 nm and are almost identical in shape. The small size ofnanoparticles makes them a suitable candidate for biomedical and pharmaceutical applications especially tocontrolled drug delivery field.Key words : Nanoparticals, PHEM, TEM, SEMIntroductionThe number of reported cases of cancer is steadily increasing in both industrialized and developing countries. Thelatest world cancer statistics indicate that the number of new cancer cases will increase to more than 15 million in2020 whereas another report issued by the World Health organization says that there are over 10 million new casesof cancer each year and over 6 million deaths annually are caused by the disease . In spite of the fact thatsignificant progress has been achieved in tumor biology, molecular genetics and in the prevention, detection andtreatment of cancer over the last few years, adequate therapy remains elusive due to late diagnosis, inadequatestrategies for addressing aggressive metastasis, and the lack of clinical procedures overcoming multi drug resistant(MDR) cancer . The integration of nanotechnology and medicine has the potential to uncover the structure andfunction of biosystems at the nanoscale level. Nanobiotechnology may provide a reliable and effective tool to treatdiseases at a molecular scale. Nanobiotechnology offers an unprecedented opportunity to rationalize delivery ofdrugs and genes to solid tumors following systemic administration . Examples of nanotechnologies applied inpharmaceutical product development include polymer-based nanoparticles, lipid-based nanoparticles (liposomes,nanoemulsions, and solid-lipid nanoparticles), self-assembling nanostructures such as micelles and dendrimers-basednanostructures among others. In recent years, much research has gone into the characterization of nanoparticles andtheir biological effects and potential applications. These include bottom-up and molecular self-assembly, biologicaleffects of naked nanoparticles and nano-safety, drug encapsulation and nanotherapeutics, and novel nanoparticles foruse in microscopy, imaging and diagnostics .To be successful a cancer treatment approach needs to overcome physiological barriers such as vascular endothelialpores, heterogeneous blood supply, heterogeneous architecture to name just a few and it strongly depends on themethod of delivery. In the past, many anticancer drugs had only limited success and had major adverse side effects.Nanoparticles have attracted considerable attention worldwide because of their unique functional characters such assmall particle size, high stability, lower toxicity, tunable hydrophilic-hydrophobic balance and the ability to bearsurface features for target specific localization, etc. Thus, polymeric nanoparticles constitute a versatile drug deliverysystem , which can potentially overcome physiological barriers, and carry the drug to specific cells or intracellularcompartments by passive or ligand-mediated targeting approaches. The use of some polymers also allows, at least inprinciple, to achieve controlled release and the sustained drug levels for longer periods of time. Numerousbiodegradable polymeric nanoparticles made of natural polymers such as proteins or polysaccharides have been triedfor drug delivery and controlled drug release. More recently the focus of such studies moved onto synthetic polymers,and much progress have been achieved in this area. Recent examples include, for example polycationic nanoparticlesfor encapsulation and controlled release of amphotericin B by Vieria and Carmona-Ribeiro ; or encapsulation of curcumin for human cancer therapy by Maitra et al.Ideally, a successful nanoparticulate system should have a high drug loading capacity thereby reducing the quantityof matrix material for administration. The drug may be bound to the nanoparticles either (i) by polymerization in thepresence of drug in most cases in the form of solution (incorporation method) or (ii) by absorbing/adsorbing the drugafter the formation of nanoparticles by incubating them in the drug solution. In the present work we set to further
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.6, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications13investigate the latter method by studying swelling and controlled release of antitumor drug doxorubicin fromsynthetic PHEMA nanoparticles. PHEMA attracted significant attention and is well documented in the literature.Many useful properties which make PHEMA attractive for a wide range of biomedical applications include highwater content, low toxicity and tissue compatibility. PHEMA has been used in applications such as soft contactlenses, drug delivery systems, kidney dialysis membranes, artificial liver support systems and nerve guidancechannels. The presence of polar groups of hydroxyl and carboxyl on each repeat unit makes this polymer compatiblewith water and the hydrophobic α-methyl groups of the backbone convey hydrolytic stability to the polymer andenhance mechanical strength of the polymer matrix. The drug chosen for this study was doxorubicin hydrochloride,which belongs to the family of anti-tumor drugs(Fig.1).. Doxorubicin is a cytotoxic anthracycline antibiotic, it iswidely used in the treatment of non-Hodkins lymphoma, acute lymphoblastic leukemia, breast carcinomas andseveral other types of cancer. We aimed to design a better PHEMA nanoparticulate delivery system for clinicaladministration of doxorubicin to achieve higher therapeutic efficacy and reduce side effects, with the overall aim todevelop effective oral chemotherapy system.Materials2-Hydroxyethyl methacrylate (HEMA) and ethylene glycol dimethacrylate (EGDMA) were purchased from SigmaAldrich Co. USA. Benzoyl peroxide (BPO) (MERCK) and polyvinyl alcohol (PVA) (Mol. Wt. 14000) (MERCK)were used as the initiator and the stabilizer, respectively. Toluene (MERCK) was used as the diluent. All chemicalswere of analytical grade.MethodsPurification of HEMAHEMA monomer was purified by using a previously reported method . The purity of distilled HEMA wasdetermined by high-pressure liquid chromatography (HPLC), [Backmen System (Gold 127)] equipped with aultraviolet detector and a 25 cm × 46 mm id separation columns ODS (C18) of 5 µm particle size. The UV detectorwas set at 217 nm. The mobile phase was methanol-water (60:40 v/v) and the flow-rate was kept at 1 mL/min. Allsamples were diluted with pure methanol to 1/1600. 10 µL samples were injected for each analysis. Samples ofknown concentrations of MAA and EGDMA were injected into the HPLC and the resultant chromatogram was usedto construct a standard curve of known concentrations vs. area under the curve. The chromatogram showed twodistinct peaks. The first peak, at 3.614 min was identified as MAA. The next peak at 5.503 min was the major peakdue to HEMA monomer. The amounts of impurities of MAA and EGDMA in the monomer samples were found tobe less than 0.01 mol% MAA and 0.001 mol% EGDMA.Preparation of PHEMA NanoparticlesPreparative methods for making nanoparticles for pharmaceutical use are broadly divided into two categories, thosebased on physiochemical properties such as phase separation and solvent evaporation, and chemical reactions such aspolymerization, and polycondensation. In the present study cross-linked PHEMA nanoparticles of definedcomposition were prepared by using a modified suspension polymerization technique.. In particular, thepolymerization was carried out in an aqueous phase containing PVA, which was used as the stabilizing agent. Themixture containing the 12.37 mM HEMA (the monomer), 1.06 mM EGDMA (the cross-linker) and 0.248 mMBz2O2 (the initiator) dispersed in toluene was added into 500 mL conical flask containing the suspension medium(200 mL aqueous PVA solution (0.5% W/V)). The reaction mixture was flushed by bubbling nitrogen and thensealed. The reaction mixture was then placed on magnetic stirrer and heated by vigorous stirring (600-700 rpm) at80°C for 2 h and then at 90°C for 1 h. The cross-linking reaction was completed within three hours. After cooling,the polymeric particles were separated from the polymerization medium by washing thrice with toluene and twicewith acetone. The collected nanoparticles were dried at room temperature to obtain the fine white powder andthereafter stored in airtight polyethylene bags. Doubly distilled water was used throughout the experiments.Characterization1.IR StudiesThe IR spectra of cross-linked PHEMA nanoparticles were recorded on a FTIR spectrophotometer (Perkin-Elmer,
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.6, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications141000 Paragon) (Shimadzu). While recording FTIR spectra KBr disc method was used for preparation of samples.2.SEM and Particle Size AnalysisMorphological studies of cross-linked PHEMA nanoparticles were performed on scanning electron micrographs(SEM). SEM observations were carried out with a Philips, 515, fine coater. Drops of the polymeric nanoparticlessuspension were placed on a graphite surface and freeze dried. The sample was then coated with gold by ion sputter.The coating was performed at 20 mA for 4 min, and observation was made at 10 KV. Nanoparticles were furthercharacterized by particle size analysis for size and size distribution. The particle size analysis of preparednanoparticles was performed on a particle size analyzer (Malvern Mastersizer 2000).Zeta potential studies were performed with a digital potentiometer (Model No. 118, EI Product, Mumbai, India). In atypical experiment 0.1 g nanoparticles were dispersed in 20 mL of respective pH solution and emf was recordedusing a compound electrode system. A similar experiment was also repeated for drug-loaded nanoparticles.Results and DiscussionThe FTIR spectra of the pure drug (doxorubicin) and loaded nanoparticles are shown in Fig. 2(a) and 2(b),respectively. The IR spectra (b) of loaded nanoparticles clearly indicate the presence of HEMA as evident from theobserved bands at 1728 cm-1(C=O stretching), 1172 cm-1(O-C-C stretching), 3556 cm-1(O-H stretching), 2951 cm-1(asymmetric stretching of methylene group) and 1454 cm-1(O-H bending) respectively. The spectra (b) also markthe presence of drug (doxorubicin) as evident from the observed bands at 1000-1260 cm-1(C-O stretching of alcohol)and 675-900 cm-1(out of plane O-H bending). The resemblance of spectra shown in Fig. 2(a) (the pure drug) and inFig. 2(b) (loaded nanoparticles) confirms the presence of drug in the loaded nanoparticles.Figure 1 FTIR spectra of PHEMA nanoparticlesSEM Analysis and Particle Size AnalysisThe SEM image of nanoparticles is shown in Fig. 2(a), which also reveals the morphology of PHEMA nanoparticles.The size of nanoparticles was estimated using SEM images. Under our experimental conditions it has been shown tovary between 100 and 300 nm. The particle size distribution curve of prepared nanoparticles is shown in Fig. 2(b).The small (defined) size of the nanocarriers’ results in the increased surface to volume ratio , enhanced frictionalforces as well as adsorption. These properties allow nanoparticles to be held in suspension and largely define theirbiological fate, toxicity and targeting ability, as well as drug loading potential, their stability and drug releaseproperties. The interaction of nanoparticles with living systems depends on their characteristic dimensions.Previously published studies proved the ability of ultra small nanoparticles to translocate throughout the body (see ξ-Potential is the difference in the electrical charge developed between the dense layers of ions surrounding theparticles and the charge of the bulk of the suspended fluid surrounding the particle; it gives information about theoverall surface charge of the particles.
Chemistry and Materials Research www.iiste.orgISSN 2224- 3224 (Print) ISSN 2225- 0956 (Online)Vol.3 No.6, 2013 - Selected from International Conference on Recent Trends in Applied Sciences with Engineering Applications15Figure 2 SEM image and particle size distribution curve of PHEMA nanoparticlesConclusionsThe prepared nanoparticles of PHEMA are will within 100 nm and may be employed as carrier for controlleddelivery of anticancer and antitumor drugs.References1.Stewart BW, Weihues P. World Cancer Report: World Health Organizaton. 2003.2. Sinha R, Kim GJ, Nie S, Shin DM. Nanotechnology in cancer therapeutics: bioconjugated nanoparticles fordrug delivery. Mol Cancer Ther. 2006; 5:1909. doi: 10.1158/1535-7163.MCT-06-0141. [PubMed] [CrossRef]3. Nie S, Xing Y, Kim GJ, Simons JW. Nanotechnology applications in cancer. Annu Rev Biomed Eng. 2007;9:257. doi: 10.1146/annurev.bioeng.9.060906.152025. [PubMed] [Cross Ref]4. Soloviev M. Nanobiotechnology today: focus on nanoparticles. J Nanobiotechnol. 2007; 5:11–13. doi:10.1186/1477-3155-5-11. [Cross Ref]5. Bajpai AK. Adsorption of a blood protein on to hydrophillic sponges based on poly (2-hydroxyethylmethacrylate) J Mater Sci Mater Med. 2004;15:583. doi:10.1023/B:JMSM.0000026380.40151.28. [PubMed] [Cross Ref]
This academic article was published by The International Institute for Science,Technology and Education (IISTE). The IISTE is a pioneer in the Open AccessPublishing service based in the U.S. and Europe. The aim of the institute isAccelerating Global Knowledge Sharing.More information about the publisher can be found in the IISTE’s homepage:http://www.iiste.orgCALL FOR PAPERSThe IISTE is currently hosting more than 30 peer-reviewed academic journals andcollaborating with academic institutions around the world. There’s no deadline forsubmission. Prospective authors of IISTE journals can find the submissioninstruction on the following page: http://www.iiste.org/Journals/The IISTE editorial team promises to the review and publish all the qualifiedsubmissions in a fast manner. All the journals articles are available online to thereaders all over the world without financial, legal, or technical barriers other thanthose inseparable from gaining access to the internet itself. Printed version of thejournals is also available upon request of readers and authors.IISTE Knowledge Sharing PartnersEBSCO, Index Copernicus, Ulrichs Periodicals Directory, JournalTOCS, PKP OpenArchives Harvester, Bielefeld Academic Search Engine, ElektronischeZeitschriftenbibliothek EZB, Open J-Gate, OCLC WorldCat, Universe DigtialLibrary , NewJour, Google Scholar